#------------------------------------------------------------------------------
#$Date: 2017-04-11 08:10:29 +0300 (Tue, 11 Apr 2017) $
#$Revision: 195328 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/22/80/7228051.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7228051
loop_
_publ_author_name
'Guo, Li-Ying'
'Li, Ying'
'Zhang, Yao'
'Li, Jian-Sheng'
'You, Wan-Sheng'
'Su, Fang'
'Zhu, Zai-Ming'
'Sang, Xiao-Jing'
'Zhang, Lan-Cui'
_publ_section_title
;
 Extended visible photosensitivity of carboxyethyltin functionalized
 polyoxometalates with common organic dyes enabling enhanced photoelectric
 performance
;
_journal_issue                   33
_journal_name_full               'RSC Adv.'
_journal_page_first              20685
_journal_paper_doi               10.1039/C7RA02353G
_journal_volume                  7
_journal_year                    2017
_chemical_formula_moiety         'C17 H79 N33 O116 P4 Sn2 W30 Zn2,13H2O'
_chemical_formula_sum            'C17 H105 N33 O129 P4 Sn2 W30 Zn2'
_chemical_formula_weight         8843.83
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2017-03-30 deposited with the CCDC.
2017-04-05 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 94.0490(10)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   13.3099(7)
_cell_length_b                   32.1189(18)
_cell_length_c                   18.9918(10)
_cell_measurement_reflns_used    8342
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      26.81
_cell_measurement_theta_min      1.66
_cell_volume                     8098.7(8)
_computing_cell_refinement       'SMART (Bruker, 2005)'
_computing_data_collection       'SMART (Bruker, 2005)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXTL (Sheldrick, 1997a)'
_computing_publication_material  SHELXTL
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997b)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0606
_diffrn_reflns_av_unetI/netI     0.0702
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       37
_diffrn_reflns_limit_k_min       -37
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            40460
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        24.999
_diffrn_reflns_theta_max         24.999
_diffrn_reflns_theta_min         1.660
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    21.946
_exptl_absorpt_correction_T_max  0.3677
_exptl_absorpt_correction_T_min  0.2400
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 2003)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.627
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             7820
_exptl_crystal_size_max          0.091
_exptl_crystal_size_mid          0.074
_exptl_crystal_size_min          0.057
_platon_squeeze_details          ' '
_refine_diff_density_max         2.016
_refine_diff_density_min         -2.665
_refine_diff_density_rms         0.330
_refine_ls_extinction_coef       0.000060(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014)'
_refine_ls_goodness_of_fit_ref   1.038
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     986
_refine_ls_number_reflns         14244
_refine_ls_number_restraints     148
_refine_ls_restrained_S_all      1.044
_refine_ls_R_factor_all          0.0754
_refine_ls_R_factor_gt           0.0455
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0415P)²+135.7654P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0997
_refine_ls_wR_factor_ref         0.1109
_reflns_Friedel_coverage         0.000
_reflns_number_gt                10318
_reflns_number_total             14244
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c7ra02353g2.cif
_cod_data_source_block           SnR-Zn-P2W15
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_database_code               7228051
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.240
_shelx_estimated_absorpt_t_max   0.368
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.05750(5) 0.17357(2) 0.80093(4) 0.02307(17) Uani 1 1 d . . . . .
W2 W -0.19287(5) 0.16141(2) 0.77977(4) 0.02228(16) Uani 1 1 d . . . . .
W3 W -0.16662(5) 0.10132(2) 0.42349(4) 0.01855(16) Uani 1 1 d . . . . .
W4 W 0.09507(5) 0.06090(2) 0.75276(4) 0.01996(16) Uani 1 1 d . . . . .
W5 W 0.11323(5) 0.11537(2) 0.44627(4) 0.01822(15) Uani 1 1 d . . . . .
W6 W 0.07217(5) 0.22724(2) 0.49316(4) 0.02218(17) Uani 1 1 d . . . . .
W7 W 0.23404(5) 0.09062(2) 0.60227(4) 0.02846(18) Uani 1 1 d . . . . .
W8 W -0.28860(5) 0.06402(2) 0.55960(4) 0.02426(17) Uani 1 1 d . . . . .
W9 W -0.32579(5) 0.17873(2) 0.60568(4) 0.02165(16) Uani 1 1 d . . . . .
W10 W -0.15564(5) 0.04864(2) 0.73212(4) 0.01960(16) Uani 1 1 d . . . . .
W11 W -0.19978(5) 0.21372(2) 0.47071(4) 0.02195(16) Uani 1 1 d . . . . .
W12 W 0.19642(5) 0.20430(2) 0.64847(4) 0.02442(17) Uani 1 1 d . . . . .
W13 W -0.09333(5) 0.30271(2) 0.57480(4) 0.02675(18) Uani 0.98 1 d . . P A 1
W13A W -0.224(3) 0.2850(13) 0.621(2) 0.025(9) Uiso 0.02 1 d . . P A 2
W14 W 0.03314(5) 0.28123(2) 0.73090(4) 0.02562(18) Uani 0.98 1 d . . P A 1
W14A W 0.035(3) 0.2986(12) 0.652(2) 0.023(8) Uiso 0.02 1 d . . P A 2
W15 W -0.22261(5) 0.26892(2) 0.71056(4) 0.02508(18) Uani 0.98 1 d . . P A 1
W15A W -0.105(3) 0.2645(11) 0.788(2) 0.025(8) Uiso 0.02 1 d . . P A 2
Sn1 Sn -0.00101(8) -0.02813(3) 0.64868(6) 0.0195(2) Uani 1 1 d . U . . .
Zn1 Zn -0.12299(15) -0.00680(6) 0.49054(12) 0.0283(5) Uani 1 1 d . . . . .
P1 P -0.0261(3) 0.07332(12) 0.5838(2) 0.0145(8) Uani 1 1 d . . . . .
P2 P -0.0674(3) 0.19716(12) 0.6345(2) 0.0150(9) Uani 1 1 d . . . . .
O1 O 0.1836(9) 0.0873(3) 0.6916(7) 0.030(3) Uani 1 1 d . . . . .
O2 O -0.4144(8) 0.0528(4) 0.5605(6) 0.029(3) Uani 1 1 d . . . . .
O3 O -0.0287(8) 0.1141(3) 0.4205(6) 0.020(2) Uani 1 1 d . . . . .
O4 O -0.2815(7) 0.0784(3) 0.4597(5) 0.017(2) Uani 1 1 d . . . . .
O5 O -0.1230(8) 0.0020(3) 0.6841(6) 0.025(3) Uani 1 1 d . . . . .
O6 O 0.1904(8) 0.2295(3) 0.5556(6) 0.020(3) Uani 1 1 d . . . . .
O7 O -0.1775(8) 0.2645(3) 0.5173(6) 0.026(3) Uani 1 1 d . . . . .
O8 O -0.0325(8) 0.0473(3) 0.7889(6) 0.023(3) Uani 1 1 d . . . . .
O9 O -0.2781(9) 0.1582(4) 0.8441(6) 0.032(3) Uani 1 1 d . . . . .
O10 O 0.0655(7) 0.0958(3) 0.5588(5) 0.018(2) Uani 1 1 d . U . . .
O11 O -0.1555(7) 0.1851(3) 0.5838(6) 0.021(3) Uani 1 1 d . . . . .
O12 O -0.1633(8) 0.1066(3) 0.7657(6) 0.022(3) Uani 1 1 d . . . . .
O13 O 0.0319(7) 0.1945(3) 0.5992(6) 0.021(3) Uani 1 1 d . . . . .
O14 O -0.0816(7) 0.2443(3) 0.6547(6) 0.021(3) Uani 1 1 d . . . . .
O15 O -0.1222(7) 0.0873(3) 0.5433(6) 0.021(3) Uani 1 1 d . . . . .
O16 O 0.1763(8) 0.0488(4) 0.8235(7) 0.032(3) Uani 1 1 d . . . . .
O17 O 0.1069(8) 0.1694(3) 0.4761(6) 0.024(3) Uani 1 1 d . . . . .
O18 O -0.2461(9) 0.2307(4) 0.3901(7) 0.034(3) Uani 1 1 d . . . . .
O19 O -0.2370(8) 0.0288(4) 0.7882(6) 0.028(3) Uani 1 1 d . . . . .
O20 O -0.1977(8) 0.1545(3) 0.4500(6) 0.021(3) Uani 1 1 d . . . . .
O21 O -0.1027(10) 0.3471(4) 0.5245(7) 0.038(3) Uani 1 1 d . . . . .
O22 O -0.2076(9) 0.1046(4) 0.3363(7) 0.033(3) Uani 1 1 d . . . . .
O23 O 0.3177(8) 0.2180(4) 0.6751(7) 0.032(3) Uani 1 1 d . . . . .
O24 O 0.1008(10) 0.3160(4) 0.7825(8) 0.044(4) Uani 1 1 d . . . . .
O25 O -0.3131(10) 0.2957(4) 0.7502(7) 0.039(3) Uani 1 1 d . . . . .
O26 O 0.0945(8) 0.0132(3) 0.7020(6) 0.021(3) Uani 1 1 d . . . . .
O27 O 0.0623(8) 0.1178(3) 0.7830(6) 0.024(3) Uani 1 1 d . . . . .
O28 O -0.0322(7) 0.0776(3) 0.6627(6) 0.019(2) Uani 1 1 d . . . . .
O29 O 0.0984(7) 0.0521(3) 0.4324(6) 0.020(3) Uani 1 1 d . . . . .
O30 O -0.2489(7) 0.0664(3) 0.6563(6) 0.021(3) Uani 1 1 d . . . . .
O31 O 0.1177(8) 0.2485(4) 0.4212(7) 0.034(3) Uani 1 1 d . . . . .
O32 O 0.1627(9) 0.1228(4) 0.3682(6) 0.031(3) Uani 1 1 d . . . . .
O33 O 0.2173(8) 0.0363(4) 0.5816(7) 0.033(3) Uani 1 1 d . . . . .
O34 O -0.2017(9) 0.2228(3) 0.7694(6) 0.026(3) Uani 1 1 d . . . . .
O35 O 0.0311(8) 0.2346(3) 0.7884(6) 0.028(3) Uani 1 1 d . . . . .
O36 O -0.2953(8) 0.2353(3) 0.6451(7) 0.029(3) Uani 1 1 d . . . . .
O37 O -0.3212(7) 0.2048(3) 0.5138(6) 0.022(3) Uani 1 1 d . . . . .
O38 O -0.2379(8) 0.0139(4) 0.5461(6) 0.029(3) Uani 1 1 d . . . . .
O39 O 0.2324(7) 0.1032(3) 0.5009(6) 0.021(3) Uani 1 1 d . . . . .
O40 O 0.1529(8) 0.1826(3) 0.7310(6) 0.025(3) Uani 1 1 d . . . . .
O41 O 0.1310(8) 0.1780(4) 0.8790(7) 0.031(3) Uani 1 1 d . . . . .
O42 O -0.0724(8) 0.1706(3) 0.8376(6) 0.025(3) Uani 1 1 d . . . . .
O43 O -0.1143(8) 0.0409(3) 0.4153(6) 0.026(3) Uani 1 1 d . . . . .
O44 O 0.1313(8) 0.2565(3) 0.6800(6) 0.026(3) Uani 1 1 d . . . . .
O45 O -0.2811(8) 0.1614(3) 0.6974(6) 0.020(2) Uani 1 1 d . . . . .
O46 O 0.2153(8) 0.1527(3) 0.6113(6) 0.025(3) Uani 1 1 d . . . . .
O47 O 0.0156(8) 0.2743(3) 0.5318(6) 0.024(3) Uani 1 1 d . . . . .
O48 O -0.0606(8) 0.2118(3) 0.4583(6) 0.021(2) Uani 1 1 d . . . . .
O49 O -0.4517(8) 0.1810(4) 0.6130(7) 0.030(3) Uani 1 1 d . . . . .
O50 O -0.3134(8) 0.1270(3) 0.5691(6) 0.022(3) Uani 1 1 d . . . . .
O51 O -0.2023(9) 0.3076(4) 0.6320(7) 0.032(3) Uani 1 1 d . U . A 1
O52 O -0.1012(8) 0.2934(4) 0.7563(6) 0.028(3) Uani 1 1 d . U . A 1
O53 O -0.0001(9) 0.3175(4) 0.6474(7) 0.030(3) Uani 1 1 d . . . A 1
O54 O 0.3633(8) 0.0914(4) 0.6226(7) 0.033(3) Uani 1 1 d . . . . .
O55 O -0.0105(9) 0.0248(3) 0.5669(6) 0.026(3) Uani 1 1 d . . . . .
O56 O -0.0643(8) 0.1726(3) 0.7022(6) 0.020(2) Uani 1 1 d . . . . .
O57 O 0.0704(17) -0.0962(7) 0.8898(13) 0.121(5) Uani 1 1 d D U . . .
O58 O -0.1005(17) -0.1160(7) 0.8574(13) 0.120(5) Uani 1 1 d D U . . .
N1 N 0.0122(15) 0.3356(7) 0.3883(11) 0.069(6) Uani 1 1 d . . . . .
H1A H -0.0124 0.3406 0.4282 0.083 Uiso 1 1 calc R U . . .
H1B H 0.0749 0.3402 0.3832 0.083 Uiso 1 1 calc R U . . .
N2 N -0.1401(16) 0.3130(9) 0.3359(15) 0.115(11) Uani 1 1 d . . . . .
H2A H -0.1694 0.3172 0.3741 0.137 Uiso 1 1 calc R U . . .
H2B H -0.1739 0.3035 0.2990 0.137 Uiso 1 1 calc R U . . .
N3 N -0.0041(15) 0.3119(8) 0.2730(13) 0.084(8) Uani 1 1 d . . . . .
H3A H -0.0395 0.3015 0.2377 0.101 Uiso 1 1 calc R U . . .
H3B H 0.0589 0.3169 0.2698 0.101 Uiso 1 1 calc R U . . .
N4 N 0.3228(14) 0.3070(7) 0.7488(11) 0.079(8) Uani 1 1 d . . . . .
H4A H 0.2947 0.3110 0.7877 0.095 Uiso 1 1 calc R U . . .
H4B H 0.2865 0.3050 0.7097 0.095 Uiso 1 1 calc R U . . .
N5 N 0.4831(16) 0.3064(7) 0.8046(11) 0.078(7) Uani 1 1 d . . . . .
H5A H 0.4591 0.3104 0.8450 0.094 Uiso 1 1 calc R U . . .
H5B H 0.5470 0.3042 0.8018 0.094 Uiso 1 1 calc R U . . .
N6 N 0.4592(19) 0.3006(8) 0.6839(14) 0.101(8) Uani 1 1 d . U . . .
H6A H 0.5230 0.3002 0.6793 0.121 Uiso 1 1 calc R U . . .
H6B H 0.4176 0.2989 0.6473 0.121 Uiso 1 1 calc R U . . .
N7 N 0.5643(18) 0.0595(9) 0.8349(15) 0.115(10) Uani 1 1 d . . . . .
H7A H 0.6289 0.0586 0.8353 0.138 Uiso 1 1 calc R U . . .
H7B H 0.5348 0.0529 0.8723 0.138 Uiso 1 1 calc R U . . .
N8 N 0.5429(13) 0.0819(7) 0.7150(11) 0.069(6) Uani 1 1 d . U . . .
H8A H 0.6065 0.0821 0.7096 0.083 Uiso 1 1 calc R U . . .
H8B H 0.5008 0.0889 0.6806 0.083 Uiso 1 1 calc R U . . .
N9 N 0.4100(16) 0.0775(8) 0.7836(12) 0.092(8) Uani 1 1 d . . . . .
H9A H 0.3857 0.0742 0.8240 0.111 Uiso 1 1 calc R U . . .
H9B H 0.3712 0.0850 0.7477 0.111 Uiso 1 1 calc R U . . .
N10 N 0.3408(11) 0.2489(6) 0.4135(10) 0.059(6) Uani 1 1 d . . . . .
H10A H 0.2803 0.2487 0.4267 0.071 Uiso 1 1 calc R U . . .
H10B H 0.3530 0.2597 0.3735 0.071 Uiso 1 1 calc R U . . .
N11 N 0.5061(11) 0.2355(5) 0.4358(10) 0.049(5) Uani 1 1 d . . . . .
H11A H 0.5547 0.2264 0.4639 0.058 Uiso 1 1 calc R U . . .
H11B H 0.5185 0.2462 0.3959 0.058 Uiso 1 1 calc R U . . .
N12 N 0.3936(13) 0.2174(6) 0.5132(10) 0.064(6) Uani 1 1 d . U . . .
H12A H 0.3327 0.2174 0.5255 0.077 Uiso 1 1 calc R U . . .
H12B H 0.4410 0.2068 0.5406 0.077 Uiso 1 1 calc R U . . .
N13 N -0.4466(11) 0.1305(6) 0.3984(11) 0.063(6) Uani 1 1 d . . . . .
H13A H -0.3997 0.1202 0.4267 0.076 Uiso 1 1 calc R U . . .
H13B H -0.4313 0.1453 0.3630 0.076 Uiso 1 1 calc R U . . .
N14 N -0.6116(12) 0.1415(6) 0.3696(11) 0.065(6) Uani 1 1 d . . . . .
H14A H -0.6737 0.1388 0.3787 0.078 Uiso 1 1 calc R U . . .
H14B H -0.5961 0.1563 0.3342 0.078 Uiso 1 1 calc R U . . .
N15 N -0.5611(12) 0.1011(7) 0.4630(11) 0.078(8) Uani 1 1 d . . . . .
H15A H -0.6224 0.0978 0.4735 0.093 Uiso 1 1 calc R U . . .
H15B H -0.5128 0.0895 0.4883 0.093 Uiso 1 1 calc R U . . .
N16 N 0.3219(18) -0.0189(8) 0.7010(18) 0.030(6) Uani 0.5 1 d . U P . .
H16A H 0.3127 -0.0312 0.7402 0.036 Uiso 0.5 1 calc R U P . .
H16B H 0.2720 -0.0071 0.6776 0.036 Uiso 0.5 1 calc R U P . .
N17 N 0.4240(19) -0.0034(8) 0.6123(18) 0.029(6) Uani 0.5 1 d . U P . .
H17A H 0.4800 -0.0054 0.5926 0.035 Uiso 0.5 1 calc R U P . .
H17B H 0.3729 0.0083 0.5902 0.035 Uiso 0.5 1 calc R U P . .
N18 N 0.488(2) -0.0356(10) 0.710(2) 0.047(6) Uani 0.5 1 d . U P . .
H18A H 0.5451 -0.0383 0.6927 0.057 Uiso 0.5 1 calc R U P . .
H18B H 0.4794 -0.0449 0.7520 0.057 Uiso 0.5 1 calc R U P . .
C1 C 0.0068(18) -0.0739(7) 0.7291(10) 0.055(3) Uani 1 1 d D U . . .
H1C H -0.0324 -0.0977 0.7118 0.066 Uiso 1 1 calc R U . . .
H1D H 0.0763 -0.0830 0.7361 0.066 Uiso 1 1 calc R U . . .
C2 C -0.029(2) -0.0621(7) 0.8007(10) 0.070(3) Uani 1 1 d D U . . .
H2C H -0.0990 -0.0544 0.7942 0.085 Uiso 1 1 calc R U . . .
H2D H 0.0084 -0.0376 0.8171 0.085 Uiso 1 1 calc R U . . .
C3 C -0.0178(17) -0.0949(8) 0.8588(13) 0.080(4) Uani 1 1 d D U . . .
C4 C -0.0478(18) 0.3207(8) 0.3337(16) 0.064(7) Uani 1 1 d . . . . .
C5 C 0.424(2) 0.3038(8) 0.7493(15) 0.071(8) Uani 1 1 d . . . . .
C6 C 0.510(2) 0.0710(10) 0.7765(18) 0.081(9) Uani 1 1 d . . . . .
C7 C 0.4137(13) 0.2332(7) 0.4540(12) 0.046(6) Uani 1 1 d . . . . .
C8 C -0.5417(13) 0.1235(7) 0.4093(12) 0.042(5) Uani 1 1 d . . . . .
C9 C 0.416(2) -0.0182(11) 0.675(2) 0.034(6) Uani 0.5 1 d . U P . .
O1W O 0.3203(17) 0.0432(7) 0.3382(13) 0.117(8) Uiso 1 1 d . . . . .
O2W O 0.259(2) 0.3190(8) 0.5837(15) 0.139(9) Uiso 1 1 d . . . . .
O3W O -0.400(2) 0.3147(10) 0.5478(18) 0.121(11) Uiso 0.75 1 d . . P . .
O4W O -0.083(3) 0.1595(12) 0.997(2) 0.118(13) Uiso 0.6 1 d . . P . .
O5W O 0.298(6) 0.099(2) 0.920(4) 0.14(3) Uiso 0.35 1 d . . P . .
O6W O -0.209(7) 0.078(3) 0.946(5) 0.11(3) Uiso 0.25 1 d . . P B 1
O7W O -0.056(6) 0.078(2) 0.937(4) 0.12(3) Uiso 0.3 1 d . . P C 2
O8W O 0.176(4) 0.1017(18) 0.976(3) 0.097(18) Uiso 0.35 1 d . . P . .
O9W O -0.286(4) -0.1003(17) 0.786(3) 0.111(18) Uiso 0.4 1 d . . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sn Sn -0.6537 1.4246 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O41 W1 O27 102.5(5) . .
O41 W1 O42 99.5(5) . .
O27 W1 O42 93.7(5) . .
O41 W1 O40 102.7(5) . .
O27 W1 O40 89.2(5) . .
O42 W1 O40 156.5(5) . .
O41 W1 O35 96.1(5) . .
O27 W1 O35 161.2(5) . .
O42 W1 O35 86.3(5) . .
O40 W1 O35 83.6(5) . .
O41 W1 O56 171.1(5) . .
O27 W1 O56 82.7(4) . .
O42 W1 O56 72.8(4) . .
O40 W1 O56 84.5(4) . .
O35 W1 O56 79.4(4) . .
O9 W2 O12 101.8(5) . .
O9 W2 O45 100.7(5) . .
O12 W2 O45 90.4(5) . .
O9 W2 O42 99.8(5) . .
O12 W2 O42 93.0(5) . .
O45 W2 O42 158.1(5) . .
O9 W2 O34 95.3(5) . .
O12 W2 O34 162.6(5) . .
O45 W2 O34 83.6(5) . .
O42 W2 O34 86.8(5) . .
O9 W2 O56 172.0(5) . .
O12 W2 O56 83.3(4) . .
O45 W2 O56 85.3(4) . .
O42 W2 O56 73.6(4) . .
O34 W2 O56 80.0(4) . .
O22 W3 O20 98.5(5) . .
O22 W3 O4 99.6(5) . .
O20 W3 O4 93.4(5) . .
O22 W3 O3 101.7(5) . .
O20 W3 O3 92.6(4) . .
O4 W3 O3 156.8(4) . .
O22 W3 O43 94.0(5) . .
O20 W3 O43 167.3(5) . .
O4 W3 O43 87.0(4) . .
O3 W3 O43 82.4(4) . .
O22 W3 O15 171.6(5) . .
O20 W3 O15 87.6(4) . .
O4 W3 O15 74.1(4) . .
O3 W3 O15 83.8(4) . .
O43 W3 O15 80.3(4) . .
O16 W4 O26 101.8(5) . .
O16 W4 O1 101.3(5) . .
O26 W4 O1 91.8(5) . .
O16 W4 O8 101.1(5) . .
O26 W4 O8 91.5(5) . .
O1 W4 O8 156.1(5) . .
O16 W4 O27 97.0(5) . .
O26 W4 O27 161.1(5) . .
O1 W4 O27 85.7(5) . .
O8 W4 O27 83.6(4) . .
O16 W4 O28 173.8(5) . .
O26 W4 O28 80.3(4) . .
O1 W4 O28 84.3(4) . .
O8 W4 O28 72.9(4) . .
O27 W4 O28 80.8(4) . .
O32 W5 O17 99.6(5) . .
O32 W5 O39 98.5(5) . .
O17 W5 O39 94.7(5) . .
O32 W5 O3 102.6(5) . .
O17 W5 O3 91.9(4) . .
O39 W5 O3 156.5(5) . .
O32 W5 O29 93.9(5) . .
O17 W5 O29 166.1(5) . .
O39 W5 O29 86.3(4) . .
O3 W5 O29 82.1(4) . .
O32 W5 O10 170.0(5) . .
O17 W5 O10 87.2(4) . .
O39 W5 O10 73.4(4) . .
O3 W5 O10 84.4(4) . .
O29 W5 O10 79.8(4) . .
O31 W6 O47 99.8(5) . .
O31 W6 O6 99.3(5) . .
O47 W6 O6 93.6(5) . .
O31 W6 O48 101.7(5) . .
O47 W6 O48 87.6(5) . .
O6 W6 O48 158.5(5) . .
O31 W6 O17 98.6(5) . .
O47 W6 O17 161.3(5) . .
O6 W6 O17 86.8(4) . .
O48 W6 O17 85.4(4) . .
O31 W6 O13 171.9(5) . .
O47 W6 O13 84.4(4) . .
O6 W6 O13 73.4(4) . .
O48 W6 O13 85.4(4) . .
O17 W6 O13 77.8(4) . .
O54 W7 O33 99.7(5) . .
O54 W7 O1 102.3(5) . .
O33 W7 O1 95.5(5) . .
O54 W7 O39 99.0(5) . .
O33 W7 O39 89.6(5) . .
O1 W7 O39 156.9(4) . .
O54 W7 O46 95.4(5) . .
O33 W7 O46 164.3(5) . .
O1 W7 O46 85.7(5) . .
O39 W7 O46 83.5(5) . .
O54 W7 O10 170.8(5) . .
O33 W7 O10 83.7(4) . .
O1 W7 O10 85.9(4) . .
O39 W7 O10 72.3(4) . .
O46 W7 O10 80.8(4) . .
O2 W8 O38 101.1(5) . .
O2 W8 O30 101.9(5) . .
O38 W8 O30 95.5(5) . .
O2 W8 O4 100.0(5) . .
O38 W8 O4 91.7(5) . .
O30 W8 O4 155.2(4) . .
O2 W8 O50 92.5(5) . .
O38 W8 O50 166.0(5) . .
O30 W8 O50 84.8(4) . .
O4 W8 O50 82.7(4) . .
O2 W8 O15 170.7(5) . .
O38 W8 O15 84.2(4) . .
O30 W8 O15 85.0(4) . .
O4 W8 O15 72.0(4) . .
O50 W8 O15 81.9(4) . .
O49 W9 O50 100.9(5) . .
O49 W9 O45 100.8(5) . .
O50 W9 O45 93.0(5) . .
O49 W9 O37 98.6(5) . .
O50 W9 O37 92.4(5) . .
O45 W9 O37 158.5(4) . .
O49 W9 O36 96.1(5) . .
O50 W9 O36 163.0(5) . .
O45 W9 O36 83.1(5) . .
O37 W9 O36 85.7(5) . .
O49 W9 O11 170.6(5) . .
O50 W9 O11 84.1(4) . .
O45 W9 O11 86.8(4) . .
O37 W9 O11 73.1(4) . .
O36 W9 O11 79.2(4) . .
O19 W10 O5 101.0(5) . .
O19 W10 O8 101.4(5) . .
O5 W10 O8 92.2(5) . .
O19 W10 O30 100.1(5) . .
O5 W10 O30 91.9(5) . .
O8 W10 O30 156.9(4) . .
O19 W10 O12 95.8(5) . .
O5 W10 O12 163.1(5) . .
O8 W10 O12 84.3(5) . .
O30 W10 O12 85.2(4) . .
O19 W10 O28 174.9(5) . .
O5 W10 O28 81.0(4) . .
O8 W10 O28 73.8(4) . .
O30 W10 O28 84.4(4) . .
O12 W10 O28 82.1(4) . .
O18 W11 O7 100.5(5) . .
O18 W11 O37 99.9(5) . .
O7 W11 O37 92.3(5) . .
O18 W11 O48 101.3(5) . .
O7 W11 O48 87.9(5) . .
O37 W11 O48 158.4(5) . .
O18 W11 O20 98.1(5) . .
O7 W11 O20 161.1(5) . .
O37 W11 O20 87.9(5) . .
O48 W11 O20 85.1(5) . .
O18 W11 O11 172.4(5) . .
O7 W11 O11 83.6(4) . .
O37 W11 O11 73.4(4) . .
O48 W11 O11 85.2(4) . .
O20 W11 O11 78.3(4) . .
O23 W12 O46 101.2(5) . .
O23 W12 O40 101.1(5) . .
O46 W12 O40 92.6(5) . .
O23 W12 O6 98.0(5) . .
O46 W12 O6 91.5(5) . .
O40 W12 O6 159.3(4) . .
O23 W12 O44 96.6(5) . .
O46 W12 O44 162.2(4) . .
O40 W12 O44 83.9(5) . .
O6 W12 O44 86.0(5) . .
O23 W12 O13 170.7(5) . .
O46 W12 O13 82.7(4) . .
O40 W12 O13 87.0(4) . .
O6 W12 O13 73.4(4) . .
O44 W12 O13 79.6(4) . .
O21 W13 O53 102.7(6) . .
O21 W13 O51 103.0(6) . .
O53 W13 O51 93.0(6) . .
O21 W13 O47 100.6(5) . .
O53 W13 O47 87.3(5) . .
O51 W13 O47 155.8(5) . .
O21 W13 O7 101.3(5) . .
O53 W13 O7 155.5(5) . .
O51 W13 O7 86.6(6) . .
O47 W13 O7 83.4(5) . .
O21 W13 O14 174.8(5) . .
O53 W13 O14 73.8(4) . .
O51 W13 O14 73.7(4) . .
O47 W13 O14 83.2(4) . .
O7 W13 O14 82.6(4) . .
O36 W13A O7 97.8(18) . .
O36 W13A O14 83.0(15) . .
O7 W13A O14 78.8(13) . .
O24 W14 O35 102.7(6) . .
O24 W14 O44 102.6(6) . .
O35 W14 O44 90.1(5) . .
O24 W14 O52 100.7(6) . .
O35 W14 O52 88.0(5) . .
O44 W14 O52 156.5(5) . .
O24 W14 O53 98.8(6) . .
O35 W14 O53 158.3(5) . .
O44 W14 O53 87.7(5) . .
O52 W14 O53 85.5(5) . .
O24 W14 O14 168.7(5) . .
O35 W14 O14 85.4(4) . .
O44 W14 O14 85.1(4) . .
O52 W14 O14 71.5(4) . .
O53 W14 O14 72.9(4) . .
O44 W14A O14 84.3(15) . .
O44 W14A O47 93.4(16) . .
O14 W14A O47 75.5(12) . .
O25 W15 O36 103.8(6) . .
O25 W15 O34 102.6(6) . .
O36 W15 O34 89.3(5) . .
O25 W15 O52 100.9(6) . .
O36 W15 O52 155.1(5) . .
O34 W15 O52 88.3(5) . .
O25 W15 O51 98.9(6) . .
O36 W15 O51 87.3(6) . .
O34 W15 O51 158.4(5) . .
O52 W15 O51 85.9(5) . .
O25 W15 O14 168.9(5) . .
O36 W15 O14 84.1(4) . .
O34 W15 O14 85.0(4) . .
O52 W15 O14 71.0(4) . .
O51 W15 O14 73.4(4) . .
O34 W15A O35 105.2(17) . .
O5 Sn1 O26 90.6(4) . .
O5 Sn1 O43 158.1(5) . 3_556
O26 Sn1 O43 87.6(4) . 3_556
O5 Sn1 O29 87.2(4) . 3_556
O26 Sn1 O29 158.7(4) . 3_556
O43 Sn1 O29 86.6(4) 3_556 3_556
O5 Sn1 C1 95.2(7) . .
O26 Sn1 C1 95.5(7) . .
O43 Sn1 C1 106.6(7) 3_556 .
O29 Sn1 C1 105.8(7) 3_556 .
O5 Sn1 O55 82.3(4) . .
O26 Sn1 O55 81.8(4) . .
O43 Sn1 O55 75.9(4) 3_556 .
O29 Sn1 O55 76.9(4) 3_556 .
C1 Sn1 O55 176.3(6) . .
O33 Zn1 O38 93.0(5) 3_556 .
O33 Zn1 O29 102.0(5) 3_556 3_556
O38 Zn1 O29 87.2(5) . 3_556
O33 Zn1 O43 86.7(5) 3_556 .
O38 Zn1 O43 101.2(5) . .
O29 Zn1 O43 167.7(4) 3_556 .
O33 Zn1 O55 91.4(5) 3_556 3_556
O38 Zn1 O55 175.1(4) . 3_556
O29 Zn1 O55 94.1(4) 3_556 3_556
O43 Zn1 O55 76.8(4) . 3_556
O33 Zn1 O55 176.5(5) 3_556 .
O38 Zn1 O55 90.5(4) . .
O29 Zn1 O55 78.3(4) 3_556 .
O43 Zn1 O55 92.5(4) . .
O55 Zn1 O55 85.1(4) 3_556 .
O15 P1 O28 111.9(6) . .
O15 P1 O10 111.6(6) . .
O28 P1 O10 111.5(6) . .
O15 P1 O55 107.7(6) . .
O28 P1 O55 107.6(6) . .
O10 P1 O55 106.2(6) . .
O56 P2 O11 112.5(6) . .
O56 P2 O13 112.0(6) . .
O11 P2 O13 111.2(6) . .
O56 P2 O14 106.9(6) . .
O11 P2 O14 107.4(6) . .
O13 P2 O14 106.5(6) . .
W7 O1 W4 148.5(6) . .
W3 O3 W5 160.1(6) . .
W3 O4 W8 123.0(5) . .
W10 O5 Sn1 141.0(6) . .
W6 O6 W12 122.0(5) . .
W11 O7 W13 152.0(6) . .
W11 O7 W13A 129.7(12) . .
W10 O8 W4 122.7(6) . .
P1 O10 W7 128.7(6) . .
P1 O10 W5 133.1(6) . .
W7 O10 W5 91.5(4) . .
P2 O11 W9 128.7(7) . .
P2 O11 W11 127.5(6) . .
W9 O11 W11 90.7(3) . .
W2 O12 W10 166.6(6) . .
P2 O13 W12 129.1(7) . .
P2 O13 W6 127.2(6) . .
W12 O13 W6 91.1(4) . .
P2 O14 W14A 128.3(12) . .
P2 O14 W13A 125.3(12) . .
W14A O14 W13A 95.9(15) . .
P2 O14 W14 123.4(6) . .
P2 O14 W15 123.0(6) . .
W14 O14 W15 93.2(4) . .
P2 O14 W13 126.7(6) . .
W14 O14 W13 90.3(3) . .
W15 O14 W13 90.2(3) . .
P1 O15 W3 133.9(6) . .
P1 O15 W8 127.0(6) . .
W3 O15 W8 90.7(3) . .
W5 O17 W6 166.7(7) . .
W3 O20 W11 166.6(7) . .
W4 O26 Sn1 142.0(6) . .
W1 O27 W4 167.0(6) . .
P1 O28 W10 127.2(6) . .
P1 O28 W4 127.3(6) . .
W10 O28 W4 89.9(4) . .
W5 O29 Zn1 126.5(5) . 3_556
W5 O29 Sn1 120.5(5) . 3_556
Zn1 O29 Sn1 108.7(5) 3_556 3_556
W8 O30 W10 147.5(6) . .
W7 O33 Zn1 131.5(7) . 3_556
W15 O34 W2 148.7(6) . .
W15A O34 W2 130.9(12) . .
W14 O35 W1 148.3(7) . .
W1 O35 W15A 127.3(12) . .
W15 O36 W9 149.2(6) . .
W13A O36 W9 139.2(14) . .
W11 O37 W9 122.6(5) . .
W8 O38 Zn1 133.0(7) . .
W5 O39 W7 122.3(5) . .
W12 O40 W1 154.9(6) . .
W2 O42 W1 123.0(6) . .
Sn1 O43 W3 119.9(5) 3_556 .
Sn1 O43 Zn1 109.5(5) 3_556 .
W3 O43 Zn1 126.6(6) . .
W14 O44 W12 148.2(7) . .
W14A O44 W12 143.9(13) . .
W9 O45 W2 154.6(6) . .
W12 O46 W7 162.0(7) . .
W6 O47 W13 151.9(6) . .
W6 O47 W14A 128.0(11) . .
W11 O48 W6 147.4(6) . .
W9 O50 W8 162.4(7) . .
W13 O51 W15 122.5(6) . .
W14 O52 W15 124.2(6) . .
W13 O53 W14 122.9(6) . .
P1 O55 Zn1 117.9(6) . 3_556
P1 O55 Zn1 118.4(6) . .
Zn1 O55 Zn1 94.9(4) 3_556 .
P1 O55 Sn1 125.7(6) . .
Zn1 O55 Sn1 97.6(4) 3_556 .
Zn1 O55 Sn1 96.0(4) . .
P2 O56 W2 129.4(6) . .
P2 O56 W1 129.7(6) . .
W2 O56 W1 89.6(4) . .
C4 N1 H1A 120.0 . .
C4 N1 H1B 120.0 . .
H1A N1 H1B 120.0 . .
C4 N2 H2A 120.0 . .
C4 N2 H2B 120.0 . .
H2A N2 H2B 120.0 . .
C4 N3 H3A 120.0 . .
C4 N3 H3B 120.0 . .
H3A N3 H3B 120.0 . .
C5 N4 H4A 120.0 . .
C5 N4 H4B 120.0 . .
H4A N4 H4B 120.0 . .
C5 N5 H5A 120.0 . .
C5 N5 H5B 120.0 . .
H5A N5 H5B 120.0 . .
C5 N6 H6A 120.0 . .
C5 N6 H6B 120.0 . .
H6A N6 H6B 120.0 . .
C6 N7 H7A 120.0 . .
C6 N7 H7B 120.0 . .
H7A N7 H7B 120.0 . .
C6 N8 H8A 120.0 . .
C6 N8 H8B 120.0 . .
H8A N8 H8B 120.0 . .
C6 N9 H9A 120.0 . .
C6 N9 H9B 120.0 . .
H9A N9 H9B 120.0 . .
C7 N10 H10A 120.0 . .
C7 N10 H10B 120.0 . .
H10A N10 H10B 120.0 . .
C7 N11 H11A 120.0 . .
C7 N11 H11B 120.0 . .
H11A N11 H11B 120.0 . .
C7 N12 H12A 120.0 . .
C7 N12 H12B 120.0 . .
H12A N12 H12B 120.0 . .
C8 N13 H13A 120.0 . .
C8 N13 H13B 120.0 . .
H13A N13 H13B 120.0 . .
C8 N14 H14A 120.0 . .
C8 N14 H14B 120.0 . .
H14A N14 H14B 120.0 . .
C8 N15 H15A 120.0 . .
C8 N15 H15B 120.0 . .
H15A N15 H15B 120.0 . .
C9 N16 H16A 120.0 . .
C9 N16 H16B 120.0 . .
H16A N16 H16B 120.0 . .
C9 N17 H17A 120.0 . .
C9 N17 H17B 120.0 . .
H17A N17 H17B 120.0 . .
C9 N18 H18A 120.0 . .
C9 N18 H18B 120.0 . .
H18A N18 H18B 120.0 . .
C2 C1 Sn1 118.1(14) . .
C2 C1 H1C 107.8 . .
Sn1 C1 H1C 107.8 . .
C2 C1 H1D 107.8 . .
Sn1 C1 H1D 107.8 . .
H1C C1 H1D 107.1 . .
C1 C2 C3 117(2) . .
C1 C2 H2C 108.0 . .
C3 C2 H2C 108.0 . .
C1 C2 H2D 108.0 . .
C3 C2 H2D 108.0 . .
H2C C2 H2D 107.2 . .
O57 C3 O58 138(2) . .
O57 C3 C2 113(2) . .
O58 C3 C2 108(2) . .
N2 C4 N1 125(3) . .
N2 C4 N3 118(3) . .
N1 C4 N3 117(2) . .
N5 C5 N4 124(2) . .
N5 C5 N6 122(3) . .
N4 C5 N6 114(3) . .
N7 C6 N8 128(3) . .
N7 C6 N9 116(3) . .
N8 C6 N9 116(3) . .
N12 C7 N10 118.8(18) . .
N12 C7 N11 121.0(18) . .
N10 C7 N11 120.1(18) . .
N15 C8 N14 122.3(18) . .
N15 C8 N13 117.9(18) . .
N14 C8 N13 119.6(19) . .
N18 C9 N17 123(4) . .
N18 C9 N16 119(4) . .
N17 C9 N16 117(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O41 1.723(12) .
W1 O27 1.826(10) .
W1 O42 1.911(11) .
W1 O40 1.924(12) .
W1 O35 2.003(11) .
W1 O56 2.391(11) .
W2 O9 1.729(12) .
W2 O12 1.827(10) .
W2 O45 1.889(10) .
W2 O42 1.901(11) .
W2 O34 1.983(10) .
W2 O56 2.363(10) .
W3 O22 1.711(13) .
W3 O20 1.835(10) .
W3 O4 1.871(10) .
W3 O3 1.886(10) .
W3 O43 2.072(11) .
W3 O15 2.354(11) .
W4 O16 1.708(12) .
W4 O26 1.811(10) .
W4 O1 1.911(13) .
W4 O8 1.927(11) .
W4 O27 1.973(10) .
W4 O28 2.381(11) .
W5 O32 1.682(12) .
W5 O17 1.830(10) .
W5 O39 1.874(10) .
W5 O3 1.918(10) .
W5 O29 2.056(10) .
W5 O10 2.357(10) .
W6 O31 1.680(12) .
W6 O47 1.862(11) .
W6 O6 1.904(11) .
W6 O48 1.908(10) .
W6 O17 1.947(10) .
W6 O13 2.366(11) .
W7 O54 1.737(11) .
W7 O33 1.797(11) .
W7 O1 1.870(13) .
W7 O39 1.967(11) .
W7 O46 2.019(11) .
W7 O10 2.341(10) .
W8 O2 1.715(11) .
W8 O38 1.771(11) .
W8 O30 1.877(11) .
W8 O4 1.961(10) .
W8 O50 2.059(10) .
W8 O15 2.379(10) .
W9 O49 1.692(11) .
W9 O50 1.813(10) .
W9 O45 1.884(11) .
W9 O37 1.941(11) .
W9 O36 1.997(11) .
W9 O11 2.342(10) .
W10 O19 1.696(11) .
W10 O5 1.821(11) .
W10 O8 1.897(11) .
W10 O30 1.920(11) .
W10 O12 1.973(10) .
W10 O28 2.367(10) .
W11 O18 1.699(12) .
W11 O7 1.868(11) .
W11 O37 1.883(10) .
W11 O48 1.885(10) .
W11 O20 1.944(10) .
W11 O11 2.371(11) .
W12 O23 1.714(11) .
W12 O46 1.824(11) .
W12 O40 1.845(12) .
W12 O6 1.937(11) .
W12 O44 2.000(11) .
W12 O13 2.341(10) .
W13 O21 1.717(12) .
W13 O53 1.851(12) .
W13 O51 1.879(12) .
W13 O47 1.941(11) .
W13 O7 1.945(11) .
W13 O14 2.411(11) .
W13A O36 1.93(4) .
W13A O7 2.21(4) .
W13A O14 2.35(4) .
W14 O24 1.702(13) .
W14 O35 1.854(12) .
W14 O44 1.857(11) .
W14 O52 1.924(11) .
W14 O53 1.992(13) .
W14 O14 2.350(10) .
W14A O44 1.91(4) .
W14A O14 2.34(4) .
W14A O47 2.41(4) .
W15 O25 1.698(12) .
W15 O36 1.864(11) .
W15 O34 1.865(11) .
W15 O52 1.946(11) .
W15 O51 1.974(13) .
W15 O14 2.358(10) .
W15A O34 1.88(4) .
W15A O35 2.04(4) .
Sn1 O5 2.045(11) .
Sn1 O26 2.054(10) .
Sn1 O43 2.064(11) 3_556
Sn1 O29 2.089(11) 3_556
Sn1 C1 2.12(2) .
Sn1 O55 2.300(11) .
Zn1 O33 2.028(11) 3_556
Zn1 O38 2.030(11) .
Zn1 O29 2.073(11) 3_556
Zn1 O43 2.104(12) .
Zn1 O55 2.225(11) 3_556
Zn1 O55 2.250(12) .
P1 O15 1.513(10) .
P1 O28 1.513(11) .
P1 O10 1.521(11) .
P1 O55 1.608(11) .
P2 O56 1.506(11) .
P2 O11 1.514(11) .
P2 O13 1.526(11) .
P2 O14 1.576(10) .
O29 Zn1 2.073(11) 3_556
O29 Sn1 2.089(11) 3_556
O33 Zn1 2.028(11) 3_556
O43 Sn1 2.064(11) 3_556
O55 Zn1 2.225(11) 3_556
O57 C3 1.276(10) .
O58 C3 1.292(10) .
N1 C4 1.35(3) .
N1 H1A 0.8600 .
N1 H1B 0.8600 .
N2 C4 1.26(3) .
N2 H2A 0.8600 .
N2 H2B 0.8600 .
N3 C4 1.36(3) .
N3 H3A 0.8600 .
N3 H3B 0.8600 .
N4 C5 1.35(3) .
N4 H4A 0.8600 .
N4 H4B 0.8600 .
N5 C5 1.27(3) .
N5 H5A 0.8600 .
N5 H5B 0.8600 .
N6 C5 1.36(3) .
N6 H6A 0.8600 .
N6 H6B 0.8600 .
N7 C6 1.34(3) .
N7 H7A 0.8600 .
N7 H7B 0.8600 .
N8 C6 1.32(3) .
N8 H8A 0.8600 .
N8 H8B 0.8600 .
N9 C6 1.36(3) .
N9 H9A 0.8600 .
N9 H9B 0.8600 .
N10 C7 1.30(2) .
N10 H10A 0.8600 .
N10 H10B 0.8600 .
N11 C7 1.30(2) .
N11 H11A 0.8600 .
N11 H11B 0.8600 .
N12 C7 1.28(2) .
N12 H12A 0.8600 .
N12 H12B 0.8600 .
N13 C8 1.32(2) .
N13 H13A 0.8600 .
N13 H13B 0.8600 .
N14 C8 1.29(2) .
N14 H14A 0.8600 .
N14 H14B 0.8600 .
N15 C8 1.29(2) .
N15 H15A 0.8600 .
N15 H15B 0.8600 .
N16 C9 1.38(4) .
N16 H16A 0.8600 .
N16 H16B 0.8600 .
N17 C9 1.30(5) .
N17 H17A 0.8600 .
N17 H17B 0.8600 .
N18 C9 1.25(5) .
N18 H18A 0.8600 .
N18 H18B 0.8600 .
C1 C2 1.518(10) .
C1 H1C 0.9700 .
C1 H1D 0.9700 .
C2 C3 1.525(10) .
C2 H2C 0.9700 .
C2 H2D 0.9700 .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N1 H1A O21 0.86 2.27 3.12(2) 169.3 .
N1 H1B O9 0.86 2.14 2.98(2) 163.9 4_665
N2 H2B O23 0.86 2.45 3.22(3) 150.2 4_565
N2 H2B O40 0.86 2.60 3.29(3) 137.5 4_565
N3 H3A O23 0.86 2.26 3.06(3) 155.9 4_565
N3 H3B O9 0.86 2.63 3.35(2) 142.2 4_665
N4 H4A O18 0.86 2.45 3.14(3) 137.1 4_666
N4 H4A O24 0.86 2.58 3.08(2) 118.1 .
N4 H4B O2W 0.86 2.44 3.22(3) 150.7 .
N4 H4B O44 0.86 2.62 3.22(2) 128.2 .
N5 H5A O48 0.86 2.30 3.07(2) 149.4 4_666
N5 H5B O25 0.86 2.18 2.99(3) 156.8 1_655
N6 H6A O25 0.86 2.49 3.20(3) 141.3 1_655
N6 H6B O2W 0.86 2.45 3.22(4) 150.1 .
N7 H7A O19 0.86 2.26 3.01(3) 145.8 1_655
N8 H8A O30 0.86 2.29 3.10(2) 156.3 1_655
N8 H8B O54 0.86 2.07 2.88(2) 156.7 .
N9 H9B O54 0.86 2.38 3.11(3) 142.9 .
N9 H9A O5W 0.86 2.37 3.16(8) 151.9 .
N10 H10A O31 0.86 2.16 2.983(19) 160.4 .
N10 H10B O34 0.86 2.13 2.90(2) 148.3 4_665
N10 H10B O42 0.86 2.56 3.21(2) 133.4 4_665
N11 H11A O37 0.86 1.97 2.822(18) 170.3 1_655
N11 H11B O35 0.86 2.15 3.00(2) 170.2 4_665
N12 H12B O49 0.86 2.08 2.94(2) 175.7 1_655
N12 H12A O6 0.86 2.05 2.90(2) 169.0 .
N13 H13A O4 0.86 2.13 2.936(18) 156.1 .
N13 H13B O24 0.86 2.04 2.90(2) 176.0 4_565
N14 H14A O32 0.86 2.23 3.06(2) 161.8 1_455
N14 H14B O52 0.86 2.19 3.01(2) 159.7 4_565
N15 H15A O39 0.86 2.04 2.890(19) 167.8 1_455
N15 H15B O2 0.86 2.18 3.02(2) 168.6 .
N16 H16B O33 0.86 2.37 3.13(3) 147.3 .
N16 H16B O26 0.86 2.52 3.20(3) 135.8 .
N17 H17A O2 0.86 2.44 3.02(3) 125.7 1_655
N17 H17B O33 0.86 2.25 3.05(3) 154.3 .
N18 H18A O1W 0.86 1.93 2.79(4) 174.6 3_656
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_4
O54 W7 O1 W4 -130.8(12) .
O33 W7 O1 W4 -29.7(13) .
O39 W7 O1 W4 72.3(18) .
O46 W7 O1 W4 134.6(12) .
O10 W7 O1 W4 53.6(12) .
O22 W3 O3 W5 -152.7(18) .
O20 W3 O3 W5 108.1(18) .
O4 W3 O3 W5 3(3) .
O43 W3 O3 W5 -60.1(18) .
O15 W3 O3 W5 20.8(18) .
O22 W3 O4 W8 178.1(6) .
O20 W3 O4 W8 -82.7(7) .
O3 W3 O4 W8 21.8(15) .
O43 W3 O4 W8 84.5(7) .
O15 W3 O4 W8 3.8(5) .
O19 W10 O5 Sn1 -135.0(10) .
O8 W10 O5 Sn1 -32.9(10) .
O30 W10 O5 Sn1 124.3(10) .
O12 W10 O5 Sn1 45(2) .
O28 W10 O5 Sn1 40.2(10) .
O18 W11 O7 W13 -130.7(14) .
O37 W11 O7 W13 128.8(14) .
O48 W11 O7 W13 -29.6(14) .
O20 W11 O7 W13 39(3) .
O11 W11 O7 W13 55.8(14) .
O18 W11 O7 W13A 130.1(14) .
O37 W11 O7 W13A 29.6(14) .
O48 W11 O7 W13A -128.8(14) .
O20 W11 O7 W13A -61(2) .
O11 W11 O7 W13A -43.4(14) .
O19 W10 O8 W4 173.8(7) .
O5 W10 O8 W4 72.0(7) .
O30 W10 O8 W4 -28.1(16) .
O12 W10 O8 W4 -91.4(7) .
O28 W10 O8 W4 -8.0(6) .
O15 P1 O10 W7 177.1(7) .
O28 P1 O10 W7 51.1(9) .
O55 P1 O10 W7 -65.8(8) .
O15 P1 O10 W5 -40.2(10) .
O28 P1 O10 W5 -166.2(7) .
O55 P1 O10 W5 76.8(9) .
O56 P2 O11 W9 49.5(9) .
O13 P2 O11 W9 176.0(6) .
O14 P2 O11 W9 -67.9(9) .
O56 P2 O11 W11 179.0(6) .
O13 P2 O11 W11 -54.5(9) .
O14 P2 O11 W11 61.6(9) .
O9 W2 O12 W10 96(3) .
O45 W2 O12 W10 -5(3) .
O42 W2 O12 W10 -163(3) .
O34 W2 O12 W10 -74(4) .
O56 W2 O12 W10 -90(3) .
O56 P2 O13 W12 -48.6(9) .
O11 P2 O13 W12 -175.5(7) .
O14 P2 O13 W12 67.9(9) .
O56 P2 O13 W6 -179.0(7) .
O11 P2 O13 W6 54.2(9) .
O14 P2 O13 W6 -62.5(9) .
O56 P2 O14 W14A 109.3(15) .
O11 P2 O14 W14A -129.8(15) .
O13 P2 O14 W14A -10.5(16) .
O56 P2 O14 W13A -114.7(14) .
O11 P2 O14 W13A 6.3(15) .
O13 P2 O14 W13A 125.5(14) .
O56 P2 O14 W14 60.0(8) .
O11 P2 O14 W14 -179.1(7) .
O13 P2 O14 W14 -59.9(8) .
O56 P2 O14 W15 -60.7(8) .
O11 P2 O14 W15 60.3(9) .
O13 P2 O14 W15 179.5(6) .
O56 P2 O14 W13 180.0(6) .
O11 P2 O14 W13 -59.0(8) .
O13 P2 O14 W13 60.2(8) .
O28 P1 O15 W3 168.2(7) .
O10 P1 O15 W3 42.4(10) .
O55 P1 O15 W3 -73.8(9) .
O28 P1 O15 W8 -53.5(9) .
O10 P1 O15 W8 -179.3(6) .
O55 P1 O15 W8 64.5(9) .
O32 W5 O17 W6 80(3) .
O39 W5 O17 W6 179(3) .
O3 W5 O17 W6 -23(3) .
O29 W5 O17 W6 -87(4) .
O10 W5 O17 W6 -108(3) .
O22 W3 O20 W11 -86(3) .
O4 W3 O20 W11 173(3) .
O3 W3 O20 W11 16(3) .
O43 W3 O20 W11 82(4) .
O15 W3 O20 W11 100(3) .
O16 W4 O26 Sn1 133.5(10) .
O1 W4 O26 Sn1 -124.6(10) .
O8 W4 O26 Sn1 31.7(10) .
O27 W4 O26 Sn1 -43(2) .
O28 W4 O26 Sn1 -40.7(9) .
O41 W1 O27 W4 -88(3) .
O42 W1 O27 W4 172(3) .
O40 W1 O27 W4 15(3) .
O35 W1 O27 W4 82(3) .
O56 W1 O27 W4 99(3) .
O15 P1 O28 W10 55.3(9) .
O10 P1 O28 W10 -178.9(6) .
O55 P1 O28 W10 -62.8(8) .
O15 P1 O28 W4 -179.6(6) .
O10 P1 O28 W4 -53.8(8) .
O55 P1 O28 W4 62.3(8) .
O2 W8 O30 W10 129.7(11) .
O38 W8 O30 W10 27.1(11) .
O4 W8 O30 W10 -78.9(15) .
O50 W8 O30 W10 -138.8(11) .
O15 W8 O30 W10 -56.6(11) .
O54 W7 O33 Zn1 -144.6(9) 3_556
O1 W7 O33 Zn1 111.9(9) 3_556
O39 W7 O33 Zn1 -45.5(9) 3_556
O46 W7 O33 Zn1 18(3) 3_556
O10 W7 O33 Zn1 26.7(8) 3_556
O25 W15 O34 W2 128.0(12) .
O36 W15 O34 W2 24.0(13) .
O52 W15 O34 W2 -131.2(13) .
O51 W15 O34 W2 -57(2) .
O14 W15 O34 W2 -60.1(12) .
O35 W15A O34 W2 20(3) .
O24 W14 O35 W1 -126.6(12) .
O44 W14 O35 W1 -23.7(12) .
O52 W14 O35 W1 132.9(12) .
O53 W14 O35 W1 60(2) .
O14 W14 O35 W1 61.3(12) .
O25 W15 O36 W9 -125.8(13) .
O34 W15 O36 W9 -23.0(13) .
O52 W15 O36 W9 61(2) .
O51 W15 O36 W9 135.7(13) .
O14 W15 O36 W9 62.0(13) .
O18 W11 O37 W9 172.8(7) .
O7 W11 O37 W9 -86.2(7) .
O48 W11 O37 W9 3.8(17) .
O20 W11 O37 W9 74.9(7) .
O11 W11 O37 W9 -3.5(6) .
O2 W8 O38 Zn1 143.5(8) .
O30 W8 O38 Zn1 -113.2(8) .
O4 W8 O38 Zn1 43.0(8) .
O50 W8 O38 Zn1 -23(3) .
O15 W8 O38 Zn1 -28.7(8) .
O32 W5 O39 W7 179.9(7) .
O17 W5 O39 W7 79.5(7) .
O3 W5 O39 W7 -26.2(15) .
O29 W5 O39 W7 -86.7(7) .
O10 W5 O39 W7 -6.2(5) .
O23 W12 O40 W1 139.2(15) .
O46 W12 O40 W1 -118.9(15) .
O6 W12 O40 W1 -18(3) .
O44 W12 O40 W1 43.6(15) .
O13 W12 O40 W1 -36.3(15) .
O24 W14 O44 W12 127.9(12) .
O35 W14 O44 W12 24.8(12) .
O52 W14 O44 W12 -60(2) .
O53 W14 O44 W12 -133.6(12) .
O14 W14 O44 W12 -60.5(11) .
O49 W9 O45 W2 -140.3(15) .
O50 W9 O45 W2 118.0(15) .
O37 W9 O45 W2 14(2) .
O36 W9 O45 W2 -45.4(15) .
O11 W9 O45 W2 34.1(14) .
O9 W2 O45 W9 140.2(15) .
O12 W2 O45 W9 -117.7(15) .
O42 W2 O45 W9 -19(2) .
O34 W2 O45 W9 46.0(15) .
O56 W2 O45 W9 -34.5(14) .
O23 W12 O46 W7 85(2) .
O40 W12 O46 W7 -17(2) .
O6 W12 O46 W7 -176(2) .
O44 W12 O46 W7 -95(2) .
O13 W12 O46 W7 -103(2) .
O31 W6 O47 W13 134.3(14) .
O6 W6 O47 W13 -125.6(14) .
O48 W6 O47 W13 32.9(14) .
O17 W6 O47 W13 -35(3) .
O13 W6 O47 W13 -52.7(14) .
O31 W6 O47 W14A -131.5(13) .
O6 W6 O47 W14A -31.4(13) .
O48 W6 O47 W14A 127.1(13) .
O17 W6 O47 W14A 59(2) .
O13 W6 O47 W14A 41.5(13) .
O18 W11 O48 W6 129.0(11) .
O7 W11 O48 W6 28.7(12) .
O37 W11 O48 W6 -62.1(19) .
O20 W11 O48 W6 -133.7(12) .
O11 W11 O48 W6 -55.0(11) .
O49 W9 O50 W8 -97(2) .
O45 W9 O50 W8 5(2) .
O37 W9 O50 W8 164(2) .
O36 W9 O50 W8 81(3) .
O11 W9 O50 W8 91(2) .
O21 W13 O51 W15 -172.3(8) .
O53 W13 O51 W15 -68.5(9) .
O47 W13 O51 W15 21.5(19) .
O7 W13 O51 W15 86.9(8) .
O14 W13 O51 W15 3.6(7) .
O21 W13 O53 W14 172.9(8) .
O51 W13 O53 W14 68.8(8) .
O47 W13 O53 W14 -86.9(8) .
O7 W13 O53 W14 -19.4(17) .
O14 W13 O53 W14 -3.2(6) .
O15 P1 O55 Zn1 115.5(7) 3_556
O28 P1 O55 Zn1 -123.8(6) 3_556
O10 P1 O55 Zn1 -4.2(8) 3_556
O15 P1 O55 Zn1 2.1(9) .
O28 P1 O55 Zn1 122.9(6) .
O10 P1 O55 Zn1 -117.6(7) .
O15 P1 O55 Sn1 -120.3(8) .
O28 P1 O55 Sn1 0.5(9) .
O10 P1 O55 Sn1 120.1(7) .
O11 P2 O56 W2 -51.1(9) .
O13 P2 O56 W2 -177.2(7) .
O14 P2 O56 W2 66.5(9) .
O11 P2 O56 W1 176.6(6) .
O13 P2 O56 W1 50.5(9) .
O14 P2 O56 W1 -65.7(8) .
Sn1 C1 C2 C3 -177.3(17) .
C1 C2 C3 O57 82(3) .
C1 C2 C3 O58 -92(3) .
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
1 -0.015 0.000 0.000 402.7 354.8
2 -0.020 0.500 0.500 402.7 353.3
